A Basic Introduction to Rheology
Total Page：16
File Type：pdf, Size：1020Kb
WHITEPAPER A Basic Introduction to Rheology RHEOLOGY AND Introduction VISCOSITY Rheometry refers to the experimental technique used to determine the rheological properties of materials; rheology being defined as the study of the flow and deformation of matter which describes the interrelation between force, deformation and time. The term rheology originates from the Greek words ‘rheo’ translating as ‘flow’ and ‘logia’ meaning ‘the study of’, although as from the definition above, rheology is as much about the deformation of solid-like materials as it is about the flow of liquid-like materials and in particular deals with the behavior of complex viscoelastic materials that show properties of both solids and liquids in response to force, deformation and time. There are a number of rheometric tests that can be performed on a rheometer to determine flow properties and viscoelastic properties of a material and it is often useful to deal with them separately. Hence for the first part of this introduction the focus will be on flow and viscosity and the tests that can be used to measure and describe the flow behavior of both simple and complex fluids. In the second part deformation and viscoelasticity will be discussed. Viscosity There are two basic types of flow, these being shear flow and extensional flow. In shear flow fluid components shear past one another while in extensional flow fluid component flowing away or towards from one other. The most common flow behavior and one that is most easily measured on a rotational rheometer or viscometer is shear flow and this viscosity introduction will focus on this behavior and how to measure it. Malvern Instruments Worldwide Sales and service centres in over 65 countries www.malvern.com/contact ©2016 Malvern Instruments Limited WHITEPAPER Shear Flow Shear flow can be depicted as layers of fluid sliding over one another with each layer moving faster than the one beneath it. The uppermost layer has maximum velocity while the bottom layer is stationary. For shear flow to take place a shear force must act on the fluid. This external force takes the form of a shear stress (σ) which is defined as the force (F) acting over a unit area (A) as shown in Figure 1. In response to this force the upper layer will move a given distance x, while the bottom layer remains stationary. Hence we have a displacement gradient across the sample (x/h) termed the shear strain (γ). For a solid which behaves like a single block of material, the strain will be finite for an applied stress – no flow is possible. However, for a fluid where the constituent components can move relative to one another, the shear strain will continue to increase for the period of applied stress. This creates a velocity gradient termed the shear rate or strain rate ( ) which is the rate of change of strain with time (dγ/dt). Figure 1 – Quantification of shear rate and shear stress for layers of fluid sliding over one another When we apply a shear stress to a fluid we are transferring momentum, indeed the shear stress is equivalent to the momentum flux or rate of momentum transfer to the upper layer of fluid. That momentum is transferred through the layers of fluid by collisions and interactions with other fluid components giving a reduction in fluid velocity and kinetic energy. The coefficient of proportionality between the shear stress and shear rate is defined as the shear viscosity or dynamic viscosity (η), which is a quantitative measure of the internal fluid friction and associated with damping or loss of kinetic energy in the system. Newtonian fluids are fluids in which the shear stress is linearly related to the shear rate and hence the viscosity is invariable with shear rate or shear stress. Typical Newtonian fluids include water, simple hydrocarbons and dilute colloidal dispersions. Non-Newtonian fluids are those where the viscosity varies as a function of the applied shear rate or shear stress. It should be noted that fluid viscosity is both pressure and temperature dependent, with viscosity generally increasing with increased pressure and decreasing temperature. Temperature is more critical than pressure in this regard with higher viscosity fluids such as asphalt or bitumen much more temperature dependent than low viscosity fluids such as water. To measure shear viscosity using a single head (stress controlled) rotational rheometer with parallel plate measuring systems, the sample is loaded between the plates at a known gap (h) as shown in Figure 2. Single head rheometers are capable of working in controlled stress or controlled rate mode which means it is 2 A Basic Introduction to Rheology WHITEPAPER possible to apply a torque and measure the rotational speed or alternatively apply a rotational speed and measure the torque required to maintain that speed. In controlled stress mode a torque is requested from the motor which translates to a force (F) acting over the surface area of the plate (A) to give a shear stress (F/A). In response to an applied shear stress a liquid like sample will flow with a shear rate dependent on its viscosity. If the measurement gap (h) is accurately known then the shear rate (V/h) can be determined from the measured angular velocity (ω) of the upper plate, which is determined by high precision position sensors, and its radius (r), since V = r ω. Other measuring systems including cone-plate and concentric cylinders are commonly used for measuring viscosity with cone- plate often preferred since shear rate is constant across the sample. The type of measuring system used and its dimensions is dependent on the sample type and its viscosity. For example, when working with large particle suspensions a cone- plate system is often not suitable. Figure 2 – Illustration showing a sample loaded between parallel plates and shear profile generated across the gap Shear thinning The most common type of non-Newtonian behavior is shear thinning or pseudoplastic flow, in which the fluid viscosity decreases with increasing shear. At low enough shear rates, shear thinning fluids will show a constant viscosity value, η0, termed the zero shear viscosity or zero shear viscosity plateau. At a critical shear rate or shear stress, a large drop in viscosity is observed, which signifies the beginning of the shear thinning region. This shear thinning region can be mathematically described by a power law relationship which appears as a linear section when viewed on a double logarithmic scale (Figure 5), which is how rheological flow curves are often presented. At very high shear rates a second constant viscosity plateau is observed, called the infinite shear viscosity plateau. This is given the symbol η∞ and can be several orders of magnitude lower than η0 depending on the degree of shear thinning. Some highly shear-thinning fluids also appear to have what is termed a yield stress, where below some critical stress the viscosity becomes infinite and hence characteristic of a solid. This type of flow response is known as plastic flow and is characterized by an ever increasing viscosity as the shear rate approaches zero (no visible plateau). Many prefer the description ‘apparent yield stress’ since some materials which appear to demonstrate yield stress behavior over a limited shear rate range may show a viscosity plateau at very low shear rates. 3 A Basic Introduction to Rheology WHITEPAPER Figure 3 - Typical flow curves for shear thinning fluids with a zero shear viscosity and an apparent yield stress Why does shear thinning occur? Shear thinning is the result of micro-structural rearrangements occurring in the plane of applied shear and is commonly observed for dispersions, including emulsions and suspensions, as well as polymer solutions and melts. An illustration of the types of shear induced orientation which can occur for various shear thinning materials is shown in Figure 4. Figure 4 - Illustration showing how different microstructures might respond to the application of shear At low shear rates materials tend to maintain an irregular order with a high zero shear viscosity (η0) resulting from particle/molecular interactions and the restorative effects of Brownian motion. In the case of yield stress materials such interactions result in network formation or jamming of dispersed elements which must be broken or unjammed for the material to flow. At shear rates or stresses high enough to overcome these effects, particles can rearrange or reorganize in to string-like layers, polymers can stretch out and align with the flow, aggregated structures can be broken down and droplets deformed from their spherical shape. A consequence of these rearrangements is a decrease in molecular/particle interaction and an increase in free space between dispersed components, which both contribute to the large drop in viscosity. η∞ is associated with the maximum degree of orientation achievable and hence the minimum 4 A Basic Introduction to Rheology WHITEPAPER attainable viscosity and is influenced largely by the solvent viscosity and related hydrodynamic forces. Model fitting The features of the flow curves shown in Figure 3 can be adequately modeled using some relatively straight forward equations. The benefits of such an approach are that it is possible to describe the shape and curvature of a flow curve through a relatively small number of fitting parameters and to predict behavior at unmeasured shear rates (although caution is needed when using extrapolated data). Three of the most common models for fitting flow curves are the Cross, Power law and Sisko models. The most applicable model largely depends on the range of the measured data or the region of the curve you would like to model (Figure 5). There are a number of other models available such as the Carreau-Yasuda model and Ellis models for example.